HAL Id: tel-02132422
https://tel.archives-ouvertes.fr/tel-02132422Submitted on 17 May 2019
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of sci-entific research documents, whether they are pub-lished or not. The documents may come from teaching and research institutions in France or abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est destinée au dépôt et à la diffusion de documents scientifiques de niveau recherche, publiés ou non, émanant des établissements d’enseignement et de recherche français ou étrangers, des laboratoires publics ou privés.
Mechanical testing procedure for local building
materials : rammed earth and laterite building stones
Abhilash Holur Narayanaswamy
To cite this version:
N°d’ordre NNT : 2016LYSET015
THESE de DOCTORAT DE L’UNIVERSITE DE LYONopérée au sein de
(L’Ecole Nationale des Travaux Publics de l’Etat) (LGCB-LTDS UMR 5513)
(Mécanique, Energétique, Génie Civil, Acoustique)
Spécialité / discipline de doctorat : Génie Civil
Soutenue publiquement le 19/12/2016, par :
(Abhilash HOLUR NARAYANASWAMY)
Mechanical Testing Procedure for Local Building
Materials: Rammed Earth and Laterite Building Stones
Devant le jury composé de :
AUBERT, Jean-Emmanuel Professor, université Toulouse III Président REDDY, B V Venkatarama Professor, Indian Institute of Science, Bangalore Rapporteur GALLIPOLI, Domenico Professor, Université de Pau et des Pays de L’Adour Rapporteur
FABBRI, Antonin Chargé de Recherche, ENTPE Examinateur
COLAS, Anne-Sophie Chargé de Recherche, IFSTTAR Examinateur
LAMARQUE, Claude-Henri HDR, ENTPE Directeur
List of publications Peer-review journal
1. H.N. Abhilash, F. McGregor , Y. Millogo, A. Fabbri, A.D. Séré, J.E. Aubert, J.C. Morel. “Physical, mechanical and hygrothermal properties of lateritic building stones (LBS) from Burkina Faso”. Construction and Building Materials, Volume 125, 30 October 2016, Pages 731–741 - http://dx.doi.org/10.1016/j.conbuildmat.2016.08.082
2. Abhilash .H.N, J.C. Morel, A. Fabbri (in press). “Shear Test Procedure for Rammed Earth”. In XIIth World Congress on Earthen Architecture, TERRA 2016, Lyon, France, 11th -14th July 2016.
v Table of contents ACKNOWLEDGMENT ... I ABSTRACT ... XI Introduction ... 1 1. 1.1. Locally available building material ... 1
1.2. Energy performance of building material ... 2
1.3. Sustainable practice ... 4
1.4. Raw earth as a building material ... 6
1.5. Mechanical properties of earthen building material ... 6
1.6. Unstabilised rammed earth (USRE) ... 8
1.6.1. History of Rammed Earth ... 8
1.6.2. Manufacturing rammed earth ... 9
1.6.3. Mechanical Performance ... 9
1.7. Laterite building stones (LBS) ... 10
2. 2.1. Selection of soil ... 11
2.1.1. Cras Sur Reyssouze (CRA)... 11
2.1.2. Dagneux ... 11
2.2. Soil particle Size Distribution ... 13
2.2.1. Discussion of soil selection based on Grain Size Distribution ... 13
2.3. Manufacture water content and Dry Density ... 16
2.3.1. Proctor Test ... 17
220.127.116.11. Test procedure ... 18
2.3.2. Importance of dry density and manufacturing moisture content ... 20
18.104.22.168. Influence of manufacturing water content on density ... 20
22.214.171.124. Influence of compaction energy on density ... 21
2.4. Suction ... 21
2.4.1. Measurement of suction ... 22
2.4.2. Procedure for suction test ... 24
2.4.3. Result ... 25
3.1. Preparation of USRE cylindrical specimens ... 29
3.1.1. For Compressive Characteristics ... 29
126.96.36.199. Large Size cylinders ... 29
188.8.131.52. Small Size Cylinders ... 31
184.108.40.206. Specimen Conditioning/ Curing... 32
3.1.2. For Tensile characteristics ... 33
3.2. Preparation of USRE Prisms ... 33
3.3. Density profile... 36
Compression Testing of Unstabilised Rammed Earth (USRE) ... 41
4. 4.1. Introduction ... 41
4.2. Experimental studies on rammed earth: a review ... 42
4.3. Objective ... 49
4.4. Experimental Protocol for USRE ... 50
4.4.1. Specimen setup ... 50
4.4.2. Extensometer ... 52
4.4.3. Linear variable displacement transducers (LVDT’s) ... 53
4.4.4. Loading Program... 54
4.4.5. Modulus of elasticity ... 56
4.4.6. Coefficient of Poisson ... 56
4.5. Result and Discussion ... 57
4.5.1. Compressive strength characteristics of CRA soil specimens ... 57
220.127.116.11. Stress strain characteristics ... 57
18.104.22.168. Influence of Compaction Energy on Compressive Strength ... 61
22.214.171.124. Influence of Dry Density on Compressive Strength ... 61
126.96.36.199. Coefficient of Poisson ... 62
188.8.131.52. Summary of CRA test ... 62
4.5.2. Compressive strength characteristics of Dagneux soil specimens ... 63
184.108.40.206. Stress strain characteristics ... 63
220.127.116.11. Influence of Compaction Energy on Compressive Strength ... 65
18.104.22.168. Influence of Dry Density on Compressive Strength ... 65
22.214.171.124. Initial tangent modulus and cyclic modulus ... 66
126.96.36.199. Coefficient of Poisson ... 68
4.6. Conclusion ... 70
5.1. Introduction ... 73
5.2. Spilt tensile test ... 74
5.2.1. Experimental procedure ... 74
5.2.2. Result and discussion ... 75
5.3. Bending test ... 77
5.3.1. Experimental procedure ... 77
5.3.2. Result and discussion ... 78
5.4. Compression test on rectangular prisms ... 81
5.4.1. Experimental procedure ... 81
5.4.2. Result and discussion ... 81
5.5. Conclusion ... 85
Experimental procedure to study interface behaviour of Unstabilised Rammed 6. Earth (USRE) ... 87
6.1. Introduction ... 87
6.2. Literature review ... 88
6.2.1. Push over test ... 88
6.2.2. Diagonal compression test and other tests on wallets ... 89
6.2.3. Shear box test ... 90
6.2.4. Tri-axial and triplet test ... 91
6.2.5. Summary ... 93
6.3. Objective ... 95
6.4. Wedge design ... 95
6.5. Digital Image Correlation (DIC) ... 97
6.6. Experimental protocol ... 98
6.6.1. Test setup ... 98
188.8.131.52. Positioning of wedges ... 98
184.108.40.206. Positioning of cameras ... 99
220.127.116.11. Specimen Surface preparation and positioning ... 101
6.6.2. Camera calibration and test run ... 102
6.6.3. Loading program ... 104
6.7. Results and discussion ... 106
6.7.1. Coulomb’s Failure Envelope ... 106
18.104.22.168. Cras Sur Reyzousse (CRA)... 106
6.7.2. Interface interlock mechanism ... 109
6.7.3. Moisture Impact ... 111
6.8. Conclusion ... 113
Experimental investigation to study compressive and flexural strength of 7. Laterite building stones (LBS) ... 115
7.1. Introduction ... 115
7.2. Materials and methods ... 116
7.2.1. Description of the tested material ... 116
7.3. Procedure and sample conditioning for the hydric tests ... 117
7.3.1. Sorption isotherms ... 117
7.3.2. Dynamic vapour sorption-desorption test ... 117
7.4. Procedure and experimental protocols of the mechanical tests ... 118
7.4.1. Sample conditioning ... 118
7.4.2. Three point bending test ... 119
7.4.3. Unconfined Compressive Test ... 120
7.5. Hydric characterization ... 121
7.5.1. Sorption-desorption isotherms ... 121
7.5.2. Moisture Buffering Value Test ... 122
7.6. Mechanical characterization ... 123
7.6.1. Three point bending test ... 123
7.6.2. Compressive Strength ... 126 7.6.3. Young’s modulus ... 128 7.6.4. Irreversible strain ... 130 7.7. Discussion ... 132 7.8. Conclusion ... 136 General Conclusion ... 137 8. 8.1. Specimen preparation and conditioning ... 137
8.2. Compressive test ... 137
8.3. Interface strength ... 139
8.4. Tensile test ... 140
8.5. Flexural test ... 140
9. Soil characteristics ... 155
Annexure - A A.1. Particle size distribution ... 155
A.1.1 Sieve Analysis ... 155
A.1.2 Sedimentation Analysis ... 155
A.2. Suction measurements ... 156
Calculation of dry density using Archimedes principle ... 159
Locally available building materials are proven energy efficient and eco-friendly, making them a sustainable building material. In the last two decades, use of raw earth as building material is augmented, owing to the environmental concerns construction industry is also reconsidering the use of raw earth, researchers on the other hand are working to understand the mechanical and dynamic behaviour of earthen buildings, yet the study of mechanical parameters possess multiple challenges due to material inert properties exposing the need of new experimental approaches to extract accurate mechanical parameters. Building techniques such as adobe, compressed earth blocks, rammed earth, and laterite building stones are on a verge of reclaiming elite position in construction industry.
In this study, experimental investigation on two naturally available building materials, unstabilised rammed earth (USRE) and laterite building stones (LBS) are carried out. The work focuses on the parameters that need to be considered in the experimental procedures, which influences the mechanical properties of USRE and LBS are seen. The locally available soils in the region of Rhone-alps, France and laterite building stones from Burkina Faso are used in this experimental campaign.
Rammed earth walls are constructed by compacting moist soil in layers, due to manufacturing technique there is a density gradient within the layer that leads to heterogeneity. On the other hand, the manufacturing parameters of the USRE such as compaction energy and manufacturing water content have a direct influence on the dry density of the material and therefore the strength. The manufacturing parameters and specimens replicating the in-situ condition are very important to understand the behaviour of USRE wall. Hence an experimental procedure to study the unconfined compressive strength, considering the influence of manufacturing parameters and specimens replicating in-situ conditions are performed along with the cyclic loading and unloading to study the elasto-plastic property of the USRE. The test procedure is performed on two different soils that are used to build USRE structures. Along with the compressive strength of USRE, the tensile strength and flexural strength are also presented by subjecting specimens under split tensile test and four point bending test.
compact that can be performed using a simple uniaxial press using inclined metallic wedges that allows rectangular prism to undergo bi-axial loading. With the help of inclined metallic wedges, shear stress and normal stress can be induced on the specimen interface allowing to obtain coulomb’s failure criteria and hence the strength properties of the interface.
1.1. Locally available building material
Naturally available materials such as earth, stones, wood etc., are the earliest materials mankind has used for dwellings. The soil and stone suitable for building constructions are abundantly available around human habitation. These locally available materials in its natural state can be used as an effective building material. Raw earth in moist state can be compacted in a wooden mould and dried under sun can be used as an earthen block. Due to its simpler technique, locally available skills can be easily employed resulting in local empowerment and low cost.
Historical evidences proves that the utilisation of raw earth (adobe) as a building material can be dated back to 10,000years (Pacheco-Torgal & Jalali, 2012). Over a period of time different techniques of using raw earth were evolved (Gallipoli, Bruno, Perlot, & Salmon, 2014). Some of the most used techniques are adobe, compressed earth blocks, rammed earth. The main constituents of the earth used in earthen buildings are clay, silt, sand and gravel, where clay acts as a binder. The mechanical parameters are largely influenced by the presence of these four constituents. Soil suitable for earth building is found in great quantities, though some soils might need additional binder due to low clay content. (Houben & Guillaud, 1994) has provided an outline of soil suitable around the world for earth building construction as shown in Figure 1-1.
Figure 1-1 Location of soil suitable for earthen buildings. Source: (Houben & Guillaud, 1994)
The rapid growth seen in the construction industry and its related activities in developed and developing countries has raised the concern of environmental pollution and depletion of natural resources (Spence & Mulligan, 1995). With increase in population and technological development, requirement for additional buildings and related activities are absolute necessary. But with conventional or modern construction practice (i.,e usage of industrial building materials), the treat for environment is high, and the embodied energy of buildings are considered to be high. In order to reduce and restore the modern construction impact, the usage of sustainable building materials is vital. The advantage of using locally available sustainable material is, it reduces transportation energy, extraction energy, and has better hygrothermal properties which reduces operational energy requirement.
The main parameters as specified by (B. V. Venkatarama Reddy, 2004) that requires attention in today’s building materials are:
Energy consumed in the manufacturing process,
Transportation of materials from quarries or industrial location to in situ,
Recycling and safe disposal,
Impact on environmental,
Long term sustainability
1.2. Energy performance of building material
materials in construction are bricks, cement, steel, aluminium, plastic products, polished stone, etc. These materials are proven to be energy intensive and contribute heavily to the global pollution. The contribution of building industry to global pollution is under scanner, the energy consumed due to extraction, manufacturing and transportation is under scrutiny. Policies on environmental issues such as reduction in CO2 emission, arresting sanctions of new quarries, obligations to rehabilitate quarry workings, and prohibition of material extraction from river beds are taken forefront (J.-C. Morel, Mesbah, Oggero, & Walker, 2001). Especially in developing countries where the construction activities are under immense development, high alert level control on exploitation of quarries, river sand, and polluting environment on a whole is given due importance.
Table 1-1 Historical development in building materials, Source: (B. V. Venkatarama Reddy, 2004)
Mud, stones, wood/thatch Prior 8000 BC
Sun dried bricks 6000 BC
Pottery products 4000 – 8000 BC Burnt bricks 4000 BC Lime 3000 BC Glass 1300 BC Iron products 1350 BC Lime-pozzolana cement 300 BC – 476 AD Aluminium 1808 AD Portland cement 1824 AD Plastics 1862
Energy consumption in buildings can be divided into two parts: (i) energy consumed due to production and transportation (embodied energy), (ii) energy consumed (required) for maintaining/servicing during the lifecycle of building. The second parameter varies from location to location depending on the climatic condition (B. V. Venkatarama Reddy, 2004).
material will have significant influence on the embodied energy. (Cabeza et al., 2013) speaks about non stabilised rammed earth having nearly zero carbon options, which can be seen from the study of venkatarama reddy (Table 1-2). In comparison with the building constructed with modern building material and rammed earth using locally available soil or stone masonry using locally available stones, a gain of more than 250% of embodied energy was observed (J.-C. Morel et al., 2001). Hence, it can be said that the raw earth without any transformation has lowest embodied energy.
Table 1-2 embodied energy in various wall, floor and roofing systems. Source: (Reddy, 2009)
Type of building element Energy per unit (GJ)
Burnt clay brick masonry (m3) 2.00 – 3.40
SMB masonry (m3) 0.50 – 0.60
Fly ash block masonry (m3) 1.00 – 1.35
Stabilised rammed earth wall (m3) 0.45 – 0.60
Non stabilised rammed earth wall (m3) 0.00 – 0.18
Reinforced concrete slab (m3) 0.80 – 0.85
Composite SMB masonry jack-arch (m3) 0.45 – 0.55
SMB filler slab (m3) 0.60 – 0.70
Non-reinforced masonry vault roof (m3) 0.45 – 0.60
The concept of energy efficient buildings means buildings build with low embodied energy and also with less energy requirement during life cycle of the building. Buildings built with raw earth has better thermal conductivity, moisture buffering and hygrothermal properties (Chabriac, 2014; Chabriac, Fabbri, Morel, Laurent, & Blanc-Gonnet, 2014; Champiré, Fabbri, Morel, Wong, & McGregor, 2016; Gallipoli et al., 2014; Ionescu, Baracu, Vlad, Necula, & Badea, 2015; Pacheco-Torgal & Jalali, 2012). Besides the energy consumption, another important parameter is recycling potential (Cabeza et al., 2013). Raw earth used in its most natural state can be recycled with no or less energy (Gallipoli et al., 2014). Considering all the above points, raw earth suits as the most efficient energy performer with high recycling potential.
1.3. Sustainable practice
natural resources and appropriate management of the building stock will contribute to saving scarce resources, reducing energy consumption, and improving environmental quality.
Considering the rapid growth in construction industry and its future prospects, the demand for construction materials will increase exponentially. To meet the demands of present and future trend in construction activities, and to ensure the sustainable practice is involved to reduce environmental impact, following parameters need to be addressed (B. V. Venkatarama Reddy, 2004):
Use of energy efficient alternative building technologies
Effective utilisation of naturally available resources
Optimal use of construction materials
Recycling building materials and its usage
Utilisation of industrial or mine wastes for manufacturing building materials
Adopting energy efficient methods in manufacturing process of building materials
Use of renewable energy and technologies to the maximum
In simple terms, the choice of building material as per OECD (as cited in(John et al., 2005) should be based on:
Harmonisation with environment
Integrated and systematic approaches
1.4. Raw earth as a building material
Unlike processed earth building materials like burnt bricks, in raw earth buildings, soil is used in its most natural state (Gallipoli et al., 2014). Simplest way of converting raw earth into building block is by compacting raw earth mixed with water in a mould, as the block dries it achieves mechanical strength. The earthen construction encompasses different manufacturing techniques, some of the commonly used techniques are called as adobe, CEB and rammed earth (Pacheco-Torgal & Jalali, 2012).
Adobe is known as the most ancient earthen construction technique, the manufacturing process of adobe is relatively simple. The adobe is manufactured by pouring moist soil (at saturation state) in a wooden mould and allowed to dry under sun; hence it is also called as sun dried bricks.
Compressed earth blocks (CEB) are the soil blocks which are compressed manually or mechanically in a metallic mould and dried in natural conditions to achieve strength. With the evolution of hydraulic machineries by adjusting water content and compaction energy, high strength compressed earth blocks are manufactured.
Rammed earth means compacting moist soil in continuous layers within a wooden or metallic formwork, the compaction process can be manual or mechanical. Another type of soil that is abundant in tropical countries is laterite; depending on the quarry laterite can be available as a loose soil or self-compacted blocks. The term laterite was coined by Buchanan in 1807 (M. D. Gidigasu, 1976). Laterites are rich in aluminium, silica, and iron oxides, its mineral and chemical composition varies based on the formation (Tardy, Kobilsek, & Paquet, 1991). It was first used as a replacement for bricks in Malabar region, India (M. D. Gidigasu, 1976). Due to its inherent properties, laterite is neither categorised as soil nor rock, hence it can be called as soft rock. In Burkina Faso, the laterite blocks used for construction of public building such as schools, churches, temples, etc., are cut from the locally available laterite deposits. Though, there no embodied energy study conducted on the laterite, considering its formation and extraction process, laterite can be categorised as the low embodied building material. Since it is naturally available and used without any transformation it can be called as a locally available raw earth building material.
1.5. Mechanical properties of earthen building material
produced guidelines for earthen construction (Pacheco-Torgal & Jalali, 2012). But they are not specific enough for modern construction practice. With growing concern regarding eco-friendly construction and evolution of the concept of sustainable construction practice, there is large community of researchers showing inclination towards studying sustainable building materials. In the last two decades, there is a tremendous growth in study of earthen building materials, research work on the study of mechanical parameters, dynamic parameters, hygrothermal parameters, durability characteristics, etc., of the soil are conducted. These studies are not limited to new construction practices, it also focuses on the conservation of ancient structures. Different experimental procedures are established to study the mechanical parameters of the earthen materials, yet there is lack of scientific information and precise procedure for manufacturing and testing specimens. Some of the mechanical parameters of adobe, CEB, rammed earth and laterite are discussed below.
In the laboratory, the mechanical characteristics such as compressive strength, tensile strength, flexural strength and shear strength of the materials is calculated by subjecting the specimens in unconfined compression test, split tensile (Brazilian) test, three point bending test and shear box or tri-axial test. The mechanical characteristics calculated in the laboratory are largely influenced based on the specimen size and shape (J. E. Aubert, Maillard, Morel, & Al Rafii, 2015). The specimen’s aspect ratio of 2 or greater than 2 is considered to be more reliable information (J.E. Aubert, Fabbri, Morel, & Maillard, 2013). Specimen preparation is a very important part of the testing procedure, specimen tested should replicate the in-situ characteristics of the material.
In unstabilised earth, clay acts as a binder and suction plays a vital role in inducing the strength (Gerard et al., 2015; P. A. Jaquin, Augarde, Gallipoli, & Toll, 2009). From the studies clay content of 14-16% is said to be optimum, which results in maximum compressive strength of the materials (Reddy, Lal, & Rao, 2007; B. V. Venkatarama Reddy & Prasanna Kumar, 2011a), but in general clay content of 10-30% is said to be acceptable (Peter Walker, Keable, Martin, & Maniatidis, 2005). If the clay content is less or to improve the mechanical characteristics of the earthen materials, cement or lime stabilisation is carried out (Gallipoli et al., 2014). Stabilisation of soil is more common in manufacturing of CEB and rammed earth. The embodied energy of the stabilised earth is higher than the unstabilised earth, but it is still lower than the other building materials (B. V. Venkatarama Reddy, Leuzinger, & Sreeram, 2014; B. V. Venkatarama Reddy, 2004). The compressive strength of cement stabilised CEB is reported as 1MPa - 2MPa (J. Morel, Pkla, & Walker, 2007; Muntohar, 2011; Reddy et al., 2007; B. V. Venkatarama Reddy & Gupta, 2006; P Walker & Stace, 1997) and that of cement stabilised rammed earth (CSRE) is 2MPa - 12MPa (Daniela Ciancio & Gibbings, 2012; Jayasinghe & Kamaladasa, 2007; Reddy & Kumar, 2009), depending on the amount of cement and clay present. The tensile strength of the earthen building material is not studied as widely as compressive strength. But from the limited research work, tensile strength of the CEB and rammed earth is reported as nearly 10% of compressive strength (T.-T. Bui et al., 2014; Gerard et al., 2015).
1.6. Unstabilised rammed earth (USRE)
The scope of this study is restricted to USRE for the soils obtained from Rhone-Alps region France and LBS obtained from Houet province in Burkina Faso.
1.6.1. History of Rammed Earth
earth (USRE) and stabilised rammed earth (SRE). Stabilisation can be done using lime or cement, depending on the need. Stabilised rammed earth construction practice is commonly seen in countries like India, Australia, (P. A. Jaquin, 2008) considering the climatic condition. Stabilisation of rammed earth in European countries was common in late 19th century (after industrialisation) (Daniela Ciancio, Jaquin, & Walker, 2013).
There are certain questions regarding the durability aspect of USRE, but from the recent studies, the deterioration of the rammed earth wallets exposed to natural climatic condition for 20years was found to be within the reasonable limits (Q. B. Bui et al., 2009). In Europe, there are certain examples of rammed earth buildings built in late 19th century and early 20th century, which are in good serviceable condition with need of some renovation (Rendell & Jauberthie, 2009). These are the classical examples of earthen building, with proper protection and care the service life of more than 100years is easily achievable.
1.6.2. Manufacturing rammed earth
Any soil with sufficient clay, silt, sand and gravel content is mixed with water and poured in a wooden or metallic formwork and compacted manually or mechanically using metallic or hydraulic rammer. The moist soil is compacted in layers forming a monolithic structure. The compacted soil is allowed to dry in natural condition; upon drying the rammed earth attains certain mechanical strength.
1.6.3. Mechanical Performance
Mechanical properties of the USRE depend on the parameters such as compaction energy, manufacturing water content, moisture within the wall (suction), soil composition. Therefore arriving at a unique mechanical property of USRE is impossible considering the variability of above mentioned parameters.
easy to handle and also resembles in-situ condition, which provides better insight of material characteristics that replicates USRE wall is important.
The main parameters that need to considered while manufacturing specimens are: soil composition, Compaction energy, and Manufacturing water content. Considering the anisotropic behaviour of rammed earth, it is also important to manufacture specimens with similar effect (i.e. ramming on the top of the layer, which leads to higher density at the top of the layer and lower density at the bottom of the layer).
Since the rammed earth structure is compacted in layers, the interface behaviour of the rammed earth plays a major role in determining the structural stability of the building under seismic condition. Hence the need to understand the behaviour of layer interfaces.
This work was influence due to the lack of experimental procedure that can recommend to study compressive, tensile, flexural and shear strengths of USRE by manufacturing specimens that replicates in-situ condition. In this study an experimental protocol to study the interface strength parameter of USRE is also proposed.
1.7. Laterite building stones (LBS)
Laterite building stones (LBS) which are available in tropical countries are a sustainable alternative material that can be easily used as a masonry construction. Though it is naturally available and poses a good mechanical strength, its scientific application as a building material was found in 1800’s (M. D. Gidigasu, 1976). The usage of LBS can be seen in developing tropical countries, but due to lack of scientific investigation on this material, its wide range application as a building material is restricted (Abdou Lawane, Pantet, Vinai, & Hugues, 2011; Unnikrishnan, Narasimhan, & Venkataramana, 2010). There are very limited research works on the LBS, some of the research works were carried out in India and Burkina Faso reported that the compressive strength of the LBS is around 1.5MPa – 4.0 MPa(A. K. Kasthurba, Santhanam, & Achyuthan, 2007; A Lawane, Vinai, Pantet, & Thomassin, 2011; Unnikrishnan et al., 2010).
2.1. Selection of soil
Any inorganic sub-soil, with limited clay content could be selected for rammed earth wall construction. Density of the rammed soil is one of the main parameter that can be controlled during manufacturing process, which has significant influence on durability and strength of the structure. Particle size distribution of any selected soil influences the density of the compacted material. The composition of unstabilised rammed earth consists of gravel & sand (45-80%), silt (10-30%) and clay (5-20%) (Daniela Ciancio et al., 2013; Delgado & Guerrero, 2007), gravels and sand forms the matrix, while clay acts as the binding material. At ideal conditions, well graded soil or any soil which satisfies fuller’s requirement of grading will have fewer voids, hence higher density when compacted at optimum condition. Excess quantity of clay increases the possibility of shrinkage damage in structure. However influence of variation in grading on physical characteristics of rammed earth is yet to be studied in detail (Maniatidis & Walker, 2003). In this chapter, location and preliminary test details of the soils used for the studying mechanical characteristics are discussed.
2.1.1. Cras Sur Reyssouze (CRA)
Cras Sur Reyssouze (CRA), is the name of the village located in [46.3092° N, 5.1664° E] Rhone-Alpes region, south east of France, as shown in Figure 2-1. In this region, there are lots of ancient rammed earth buildings in need of renovation and few new rammed earth buildings being constructed. The soil used in this study is extracted from an ancient building wall which was demolished during renovation.
Dagneux is another soil used in this study, which is also located [45.8508° N, 5.0753° E] in the Rhone-Alps Region, south-east of France, as shown in Figure 2-1. As said earlier in this village too there is lot of ancient rammed earth construction. The soil samples fabricated in this study are extracted from the ancient rammed earth building, not in use anymore.
and also useful for new construction activities. The other advantage of using this soil in our study is its maximum granular size is less than 10mm, which will be easy to standardize the laboratory results for actual field conditions.
Figure 2-1 Location of the soils used in this study
Figure 2-2 Particle Size Distribution of soil and maximum and minimum grain size distribution of soil for civil engineering purpose recommended by (BS 1377-2, 1990)
Sieve Size (mm)
CRA Dagneux BS 1377 Max BS 1377 Min
2.2. Soil particle Size Distribution
Particle size distribution of both soils (CRA and Dagneux) are carried out in accordance to British standard (BS 1377-2, 1990). Wet sieve method is adopted for removing clay and silt fraction from gravel and sand, later using various sieves, gravel and sand quantities is calculated. While clay and silt fractions are obtained through sedimentation test using hydrometer. By combining both sieve results and sedimentation results, particle size distribution of the soil is plotted in Figure 2-2. Both soils are out of the range given by (BS 1377-2, 1990), whereas this soils enabled to build safe houses lasting for more than 70 years with low maintenance. It is worth rejecting recommended maximum and minimum grain size distribution of soil, because they don’t take into account the great variability of possible soils and techniques. Moreover these limits are against sustainability because they may discard a local suitable local soil which is favourable to decrease the impact on environment (Morel et al. 2001).
2.2.1. Discussion of soil selection based on Grain Size Distribution
Some guideline and technical document recommends the selection of soil with respect to grain size distribution and on the percentage of clay content present in the soil. In Table 2-1, from (Daniela Ciancio et al., 2013; Delgado & Guerrero, 2007; Gomes et al., 2014; Maniatidis & Walker, 2003; Peter Walker et al., 2005) studies, the recommendations of lower and upper limit of grains distributed in a soil for earth buildings are given. From earlier study and recommendations, in general it could be seen that soil with clay content varying from as low as 5% to as high as 30% is acceptable. Except (Alley, 1948 as cited in, Maniatidis & Walker, 2003) who proposed higher silt content (50-80%) and lower sand and gravel content (10-20%), other works commonly agree with minimum and maximum silt content of 10% and 30% respectively, along with the minimum and maximum sand and gravel content of 40% and 80% respectively. Studies which does not recommend silt content in the soil, proposes high quantity of sand and gravel content with lower and upper limit as 65% and 80% respectively, it should also be noted that when silt is not present an increased clay content is advised with minimum being 20% and 35% as maximum. Some of the works recommends sand and gravel quantities separately, though not all the earlier studies points out the maximum gravel size considered, in general it could be seen most of the authors consider 20mm down as the maximum gravel size.
quota of clay required for obtaining a good mix. CRA satisfies the silt, sand and gravel content recommended by many normative and technical standards. But Dagneux, is high with silt presence (65%), and low with sand and gravel content, it represents the limits presented by (Alley, 1948; as cited in Maniatidis & Walker, 2003) in his work. Both the soils chosen for this study does not obey the limits stated by British standards (BS 1377-2, 1990) for earth constructions, but still they are actively used for earth wall construction from a very long period.
Table 2-1 Particle size limits proposed by various study
Author/ Name Clay Silt Sand & Gravel
(Peter Walker et al., 2005) 5-20% 10-30% 45-80%
(Alley, 1948) 1 25-30% 50-80% 10-20%
(Schrader, 1981)1 20-30% - 70-80%
(McHenry, 1984)1 30-35% - 65-70%
(Norton, 1986)1 10-25% 15-30% 45-75%
(Houben & Guillaud, 1994)1 0-20% 10-30% 45-75%
(Radanovic, 1996)1 30-35% - 65-75%
(SAZS 724:2001, n.d.)1 5-15% 15-30% 50-70%
(Bolton, 2001) 5-15% 15-30% 40-70%
British standard2 N.A* N.A* N.A*
HB-195, (Peter Walker & Standards
Australia, 2002)2 5-20% 10-30% 45-75%
Bulletin 52 N.A* N.A* N.A*
NZ standard for earthen construction N.A* N.A* N.A*
MOPT (1992)3, spain 5-26% NA* NA*
IETcc (1971)3 10-40% 20-40% 10-20%
(McHenry, 1984)3 15% 32% 30% ( Sand) +
Smith and Austin (1996)3, New Mexico 4-15% 40% 60-80%
Gomes & Folque (1953)4 15-31% 7-17% 28-51% (Sand) +
0-33% (Gravel) Doat, et al. (1979)4, CraTerre 15-25% 20-35% 40-50% (Sand) +
0-15% (Gravel) Keable (1996)4 5-15% 15-30% 50-70% Keefe (2005)4 7-15% 10-18% 45% (Sand) + 30% (Gravel) CRA 17% 28% 55% Dagneux 20% 65% 15%
*Note: N.A – Not Available
Table 2-2 Grain Size of soils considered in this project
1 As cited in (Maniatidis & Walker, 2003) 2 As cited in (Daniela Ciancio et al., 2013) 3 As cited in ((Delgado & Guerrero, 2007) 4
Grain's CRA [%] Dagneux [%]
Gravel (60-2mm) Coarse (60-20mm) 0 55% 0 15% Medium (20-6mm) 0 0 Fine (6-2mm) 1 0,5 Sand (2-0,06mm) Coarse (2-0,6mm) 4 1 Medium (0,6-0,2mm) 30 2,5 Fine (0,2-0,06mm) 20 11 Silt (60µm-2µm) Coarse (60-20µm) 11 28% 42 65% Medium (20-6µm) 11 13,7 Fine (6-2µm) 6 9,3 Clay (<2µm) <2µm 17% 20%
2.3. Manufacture water content and Dry Density
Density of the construction material is an indicative factor of material durability and strength. Density of the oven dry (at 100-110°C) material is termed as Dry density and in general it is measured in g/cc or kg/m3. For a given soil at known compaction energy, dry density of the soil varies with increase in the water content. It may reach a point where the soil is no more compressible as water completely occupies voids. During the compaction process if soil achieves its maximum dry density (MDD) this water content is called as ‘optimum moisture content’ (OMC) or optimum water content (OWC) for a given compaction energy. For the case of rammed earth, the Proctor test is commonly adopted (Maniatidis & Walker, 2003) to measure the maximum dry density and optimum moisture content for a given compaction energy.
From earlier studies, it is understood that dry density of rammed earth varies from 1.7 to 2.2g/cc (Araki et al., 2011; Q. Bui, Morel, Hans, & Walker, 2014; Cheah, Walker, Heath, & Morgan, 2012; Maniatidis & Walker, 2003). It is widely known that the material strength increases with increase in dry density (A W Bruno, Gallipoli, Perlot, Mendes, & Salmon, n.d.; B. V. Venkatarama Reddy & Prasanna Kumar, 2011b), but owing to lack of more reliable scientific studies on USRE, there is a need to understand the influence of dry density on the USRE wall.
compaction effort adopted at site and proctor test is always difficult, however Proctor compaction method still serves as the reliable scientifically proven procedure to investigate compaction energy and manufacturing water content of the USRE.
It goes without saying density of compacted soil varies from soil to soil with change in particle size distribution. It is absolutely necessary to know the target dry density to be achieved for the rammed earth wall in construction.
2.3.1. Proctor Test
The term proctor is coined after R R Proctor, who in 1933 showed that the dry density of a soil for a given compactive effort depends on the amount of moisture present in the soil at the time of compaction.
General practice involves proctor test on soil with standard (600kN.m/m3) and modified (2733kN.m/m3) compaction energy. Proctor test on the soils studied in this work is carried out in accordance to (ASTM D1557-12, 2012; ASTM D698-12e2, 2012).
Figure 2-3 Proctor Testing Instruments
22.214.171.124. Test procedure
Table 2-3 Compaction Details of Proctor Test
Standard (E-S) Modified (E-M) E3
Weight of Hammer 2.5kg 4.54kg 4.54kg
Height of fall 305 457 457
N° of Blows 56 56 56
N° of Layers 3 5 3
Compaction Energy 600kN.m/m3 2731kN.m/m3 1639kN.m/m3
Dry density [γd] of the soil is calculated by using the relation, 𝛾𝑑 = 1+𝜔𝛾 , where [γ]
is bulk density and [ω] is moisture content of the soil. The variation of dry density with respect to increase in moisture content of the soil at compaction is given in Figure 2-4, in which both the soils (CRA & Dagneux) are represented. As said earlier it can be seen that the optimum moisture content of the soil decreases and maximum dry density increases with increase in compaction energy, the optimum moisture content and dry density for both the soils at different energies is given in the Table 2-4.
Figure 2-4 Optimum Moisture Content - Maximum Dry Density (Proctor)
Table 2-4 Optimum moisture content and maximum dry density of soils
Soil CRA Dagneux
Compaction Energy, kN.m/m3 600 - 2731 600 1639 2731
Optimum Moisture Content [ω], % 10.5 - 9.0 13.5 11.5 11.0
2.3.2. Importance of dry density and manufacturing moisture content
As said earlier, density of the material defines the strength and durability of the material, material with a high density will have better mechanical characteristics, but the influence of density on mechanical parameter of unstabilised rammed earth is not yet studied in detail. From proctor results, it can be seen that with different energies the density achieved is different, however it also depends on the manufacturing water content, defining the parameters such as manufacturing water content and compaction energy for a soil is very difficult, moreover in the field, measuring water content and compaction energy is difficult too. With different practitioners and depending the method they adopt to construct a rammed earth, density achieved will vary, (Quoc-Bao, 2008) in this work identifies masons using pneumatic rammers compact rammed earth with an energy of 1900kN.m/m3.
126.96.36.199. Influence of manufacturing water content on density
In Figure 2-5, density variation with manufacturing water content and compaction energy is shown. On the left side of optimum moisture content, dry density for any compaction energy increasing until it reaches optimum moisture, which is also called as the ‘dry side of OMC’. On the right side of optimum moisture content, density of the material decreases with increase in moisture, this portion is also called as ‘wet side of OMC’. From the Figure 2-5, it can be seen that point a and aˈ have same density [γa] for a
Figure 2-5 Concept of Manufacturing water content and achieved dry density
188.8.131.52. Influence of compaction energy on density
In Figure 2-5, it can also be seen that, points a and c, b and e, bˈ and d, share same manufacturing water content, but has different dry densities, it is due to difference in the compaction effort. It is to say if there is change in compaction energy for given water content, there will be change in density achieved. Hence studying the influence of density and compaction energy on mechanical parameters of unstabilised rammed earth is important. Answering these questions is vital for better practice of unstabilised rammed earth construction. To analyse the impact of different compaction energy and density on the mechanical parameters, the cylindrical specimens at different compaction energies are manufactured and subjected to compression test. In the following chapters specimen manufacturing and mechanical strength of USRE will be discussed.
between the soil particles (P. A. Jaquin et al., 2009), which increases apparent cohesion thereby contributing to strength (Nowamooz & Chazallon, 2011). Suction increases with decrease in moisture, similarly the strength and modulus of USRE increases with decrease in moisture (Araki et al., 2011; Q. Bui et al., 2014; Gerard et al., 2015).
2.4.1. Measurement of suction
Measurement of suction can be classified into two main categories; (i) Direct method for measuring matric suction, and
(ii) Indirect method for measuring matric, osmotic and total suction
Direct suction measurement technique includes: axis- transition technique, tensiometer and suction probe methods. Indirect suction measurement technique (for matric suction) includes: time domain reflectometry (TDR), electrical conductivity sensors, thermal conductivity sensor (TCS) and in-contact filter paper technique methods (Pan, Qing, & Pei-yong, 2010).
Filter paper technique is considered to be easily affordable and has wide range of suction measurement possibility (Bulut, 1996; Pan et al., 2010). Using filter paper method, both total suction and matric suction can be studied. The total suction of the soil can be studied by suspending the filter paper (without physical contact) with the specimen in a sealed contained. The matric suction of the soil can be calculated by bringing filter paper in contact with the specimen surface, thereby allowing direct contact for liquid phase and solutes to exchange freely. In this study, only matric suction is studied by using in-contact filter paper.
2007) depending on the type of suction and method used. The calibration curves widely accepted is presented in Table 2-5 (source (Bicalho et al., 2007)). It is recommended to establish a calibration curve for the Whatman 42 filter paper available in each lab. At ENTPE, Lyon, the calibration curve for Whatman 42 filter paper using salt solutions in accordance with the (ASTM D5298-03, 2003) was established by (SOUDANI, 2016) (Figure 9-1 - annexure). The suction value for Whatman 42 filter paper can be calculated from the equation 𝑆 = 5.2473 − 0.1241 𝑤 , which is obtained through calibration chart established by (SOUDANI, 2016) in ENTPE lab. Where S is suction in log kPa, w is the filter paper water content.
Figure 2-6 Calibration suction-water content curves for wetting of filter paper (source: (ASTM
Table 2-5 Calibrations curves for Whatman 42 filter paper (source: (Bicalho et al., 2007) )
Reference Suction W (%) range Log10 (suction), kPa
ASTM D5298 Total & Matric W < 45.3 5.327 - 0.0779 w
ASTM D5298 Total & Matric W > 45.3 2.412 – 0.0135 w
Chandler & Gutierrez (1986) Matric (*) 2.85 – 0.0622 w
Chandler et al. (1992) Matric W < 47 4.842 – 0.0622 w
Chandler et al. (1992) Matric W > 47 6.050 – 2.48 log w
Oliveira & Marinho (2006) Total & Matric W < 33 4.83 – 0.0839 w Oliveira & Marinho (2006) Total & Matric W > 33 2.57 – 0.0154 w (SOUDANI, 2016) Total & Matric W < 20 5.247 – 0.124 w
Note: w = Gravimetric water content and (*) suction range (80-6000kPa)
2.4.2. Procedure for suction test
In this study, the experimental procedure in accordance with (ASTM D5298-03, 2003) was followed. Cylindrical specimens of dimensions 100mm in diameter and 60mm in height were used. In order to speed up the experiment, cylindrical specimens with 4%, 6% and 8% water contents were manufactured, thereby reducing time taken in drying process. Each set of moisture content had 4 cylindrical specimens. The diameter of the Whatman 42 filter paper to be placed in-contact with the soil surface is curtailed and sandwiched in-between two filter paper of same make as shown in Figure 2-7. Before commencing the experiment, the air dry weight of the curtailed Whatman 42 filter paper is weighed to the precision of 0.001g, and the weight of the moist soil specimen is weighed with precision 0.01g.
soil specimens are reused to measure suction values at less than 4% soil water content. The oven dry soil specimens are categorised into three groups, one group of specimens are placed in climatic controlled room at 23° C and 50% RH, the second group of specimens are placed in air tight box with salt solution to maintain a RH of 23% at 23° C, and finally the third group of specimens are used as over dry state. These three groups of specimens had a soil moisture content of around 2% and 1% and 0% (oven dry state).
Figure 2-7 Filter paper arrangement
Table 2-6 suction calibration equations used for CRA and Dagneux soil
Reference Suction W (%) range Log10 (suction), kPa
ASTM D5298 Total & Matric W < 45.3 5.327 – 0.0779 w
Chandler et al. (1992) Matric W < 47 4.842 – 0.0622 w
Oliveira & Marinho (2006) Total & Matric W < 33 4.83 – 0.0839 w
Lucile (ENTPE, Lab) Matric - 5.2473 - 0.1241 w
Note: ‘w’ is the filter paper water content
The suction values are calculated with respect to the filter paper water content, but in the analysis gain of suction is expressed with respect to change in soil water content. The suction values of CRA and Dagneux soil specimens with respect to the calibration of (SOUDANI, 2016), ENTPE is presented in Figure 2-8. The soil suction increases with decrease in soil water content for both the soils examined, this is in agreement with (Q. Bui et al., 2014; Daniela Ciancio et al., 2013; Gerard et al., 2015; P. A. Jaquin et al., 2009; Nowamooz & Chazallon, 2011). Hence suction contributes to the gain in strength of USRE with decrease in moisture content. Considering the significant difference in suction calibration values, to obtain a good correlation, it is recommended to establish a calibration chart for the batch of filter paper used in the lab.
Sample Preparation and Conditioning 3.
In this section, different soil specimens manufactured for studying suction, compressive strength, tensile strength, shear strength, and flexural strength of the material will be elaborated.
3.1. Preparation of USRE cylindrical specimens 3.1.1. For Compressive Characteristics
Cras-sur-Reyssouze and Dagneux soils are extracted from an ancient building which was demolished during renovation work. These were unstabilised walls, and large cubes were transported to laboratory. As a preliminary work, soils are manually crushed using hammer, to obtain maximum grain size of 10mm, crushed soils grain size were roughly estimated and passed in a mechanical crusher with maximum size of 10mm.
Soil is air dried before estimating the initial moisture content present in the lot. Designed water content is calculated and added to the soil and mixed well until the homogeneous mix is achieved, depending on the quantity of soil mixed, manual or mechanical stirrer is used, if the quantity of soil mixed is less than 50kg then hand mixing is preferred. Homogeneous wet soil is then transferred to air tight plastic bags and preserved for 24hrs before using them to manufacture specimens; this will ensure that the water equilibrium is achieved within the soil mix.
184.108.40.206. Large Size cylinders
Figure 3-1 Cras-Sur Reyssouze Cylindrical Specimens: (a) E3 compaction energy, (b) Standard Energy & (c) Modified Energy
To obtain different dry densities [ϒd] of the rammed earth soil specimens, soil was
mixed with different water contents referring to OMC obtained from the proctor test, which can be classified as dry side of OMC and wet side of OMC. Specimens C3 and C5 are manufactured at different water contents, but the dry densities achieved are same for compaction energy of 2730kN.m/m3, and also C6 and C8 are manufactured on similar lines for compaction energy of 990kN.m/m3, specimen details are given in the Table 3-1.
Also another important criterion considered is to manufacture specimens by varying compaction energy for same manufacturing water content. C2 and C8 are manufacture at 9.5% manufacturing water content for 600kN.m/m3 and 990kN.m/m3 compaction energy respectively. C4 and C5 are manufactured at 10.2% manufacturing water content for 600kN.m/m3 and 2730kN.m/m3 compaction energy respectively.
Table 3-1 Manufactured Specimen Details of CRA soil
Compaction Energy, [kN.m/m3] Specimen N° Of Layers Manufacturing Water Content Dry Density, [g/cc] OMC 600 C2 C4 3 3 9.6% 10.2% 1.89 1.87 10.5% 956 C1 3 5.7% 1.86 - 990 C6 C8 5 5 10.8% 9.4% 1.95 1.95 10% 2730 C3 C5 5 5 11.1% 10.2% 2.02 2.02 9%
Manufacturing water content of the soil specimens are calculated in accordance with (ASTM-D-2216-98, 1998), a portion of soil used for compaction layers is taken for determining water content. Water content is calculated by calculating the weight difference of the moist soil and oven dried soil at 100-105°c after 48hrs.
The metallic cylindrical mould used for manufacturing specimens were released as soon as the final layer is compacted, precautions were taken not to damage the specimen during release of compaction mould.
220.127.116.11. Small Size Cylinders
then filled with sand, such that the cardboard is not displaced or broken due to the energy generated during ramming process.
Figure 3-2 Small Cylinders of dimension 110mm (diameter) and 220mm (height), (a) Cylindrical cardboard tube (formwork), (b) Manufactured specimen
Table 3-2 Small Cylindrical Specimens - Manufacturing Conditions
Compaction Energy, [kN.m/m3] Specimen’s Manufacturing Water Content, [%] Dry Density, [g/cc] N° of Specimens 600 D1 10.6% 1.77 1 970 D2 9.9% 1.82 4 2580 D3 11.2% 1.96 3
18.104.22.168. Specimen Conditioning/ Curing
during drying process, so that the moisture state of all the specimens are identical. Specimens were subjected to test, when the weight difference of two consecutive readings (24hours) was constant (± 0.01g).
3.1.2. For Tensile characteristics
Cylindrical specimens similar to large size cylinders are manufactured to study the tensile strength of both CRA and Dagneux soils. Specimens are manufactured in a cylindrical cardboard tube of dimension 160mm in diameter and 320mm in height, specimens were rammed by placing the cardboard tube in a wooden box filled with sand such that the external surface of the tube is covered by the sand. Weighed quantity of moist soil for each layer is poured into the cardboard tube and manual compacted using a metallic rammer (as shown in Figure 3-3) until the desired layer thickness of 60mm (± 2mm) is achieved. Three specimens for each soil was manufactured and stored in the climate camber at 25°C and 60% relative humidity.
Figure 3-3 Manual Compaction of Cylindrical (Large) Specimens (a) Manufacturing Set up, (b) Rammer
3.2. Preparation of USRE Prisms
study, only two layered rectangular specimens were manufactured and tested, with layer thickness of 60mm (+/-2mm) each.
All the rectangular prisms are manually compacted in a wooden box fabricated in the laboratory as shown in the Figure 3-4 (a). Using a metallic rammer as shown in the Figure 3-4 (b), weighed moist mass of soil for each layer is rammed until the desired layer thickness of 60mm is achieved. In order to improve the cohesion force of the layer interface, for some of the specimens, forced indentation (as shown in Figure 3-6) was made on the layer interface surface before ramming the top layer, this layer indentation or surface scratching was done only for Dagneux soil. For CRA and remaining Dagneux specimens, no surface indentation was made; hence it has a smooth layer interface surface.
Since manual compaction was adopted, the compaction energy was not monitored, but the manufacturing water content of the soil was controlled while mixing. The moisture content of the moist soil is measured for each specimen manufactured. Moist soil is prepared similar to as explained in the above section. Weighed moist soil rammed for each layer was calculated according to the desired dry density to be achieved. The manufacturing details of the rectangular prism specimens manufactured for studying interface shear properties are given in the Table 3-3.
Failure of prism specimens tested for interface shear strength test are due to delamination of interface, thereby two layers of rammed earth prism are obtained after the test. Care has been taken to select specimen layers without damage. Specimens without damage are later used to study the compressive strength and flexural strength of the prisms. Prism specimens (layer) with dimension of 210×120×60 mm (obtained from 30°inclination) are used for compression test, and 330×120×60 mm (obtained from 20° inclination) is used for flexural test.
Figure 3-4 (a) Wooden Formwork used for Ramming Prism Specimens, (b) Manual Metallic Rammer
Figure 3-5 Specimens used for Shear Test (a) for 45° Inclination, (b) for 30° Inclination, (c) for 20° Inclination
Table 3-3 Rectangular Prism Specimen Manufacturing Details
Soil Angle of inclination tested N° of Specimens Manufactured water content Dry Density, g/cc CRA 20° 3 9.20 1.70 30° 3 9.80 1.88 45° 3 9.20 1.94 Dagneux 20° 3 10.63 1.72 30° 5 9.52 1.84 30°(Indentation) 7 10.95 1.81 45° 6 10.70 1.85 45°(Indentation) 4 10.65 1.82 3.3. Density profile
Figure 3-7 representation of variation of density within the layer
To analyse the variation of densities within the layers, cylindrical specimens manufactured at three different compaction energies are considered. Layers of the cylindrical specimens were delaminated and each layer is cut in the middle, such that top and bottom part of the layer is extracted as shown in Figure 3-8. As a next step, three samples from top and bottom part are taken for calculating the densities within the layer. The densities of the samples extracted within the layers are calculated based on the Archimedes principle.
Figure 3-8 graphical explanation of specimen extraction for density calculation
The dry density of the top and bottom parts of the layer is calculated for all 5 layers, and the average dry density of top and bottom layer is taken for analysis. In case of CRA soil specimen manufactured at 600kN.m/m3, only three layers are investigated. The variation of dry density for CRA and Dagneux specimens is given in Table 3-4. The difference in dry density within the layer decreases with increase in compaction effort, leading to more homogenised layer formation.
Table 3-4 Density variation of CRA and Dagneux soil specimens
Soil CRA Dagneux
Compaction energy 600 990 2730 600 970 2580
Dry density, g/cc Top 2.13 2.11 2.15 1.95 2 2.06
Bottom 1.9 2.02 2.13 1.70 1.84 2.01
Difference in dry density,
g/cc 0.23 0.09 0.02 0.25 0.16 0.05
% variation from top to
Compression Testing of Unstabilised Rammed Earth (USRE) 4.
Compressive strength is one of the most important parameter considered in design guidelines; it serves as the basic mechanical parameters in selection of material for building construction (J. Morel et al., 2007; B. V. Venkatarama Reddy & Prasanna Kumar, 2011a). The compressive strength of USRE is considered to be in between 0.5MPa – 4 MPa (Daniela Ciancio & Jaquin, 2011; Maniatidis & Walker, 2003) and the other earthen building material such as CEB was reported to vary in between 2-15MPa depending on the stabilisation (Deboucha & Hashim, 2011; J. Morel et al., 2007; Muntohar, 2011; Reddy et al., 2007; B. V. Venkatarama Reddy & Gupta, 2006, 2008; P Walker & Stace, 1997). The study of (A W Bruno et al., n.d.), showed that the mechanical parameters of unstabilised CEB can be enhanced by increasing the compaction effort. The strength of the CEB’s compacted at high pressures were found to be in between 4.2-10MPa, this kind of strength is similar to that of stabilised CEB’s. Hence the influence of the compaction energy on the earthen building materials has a very important role in design. In case of CEB’s, compaction on top and bottom surface of the block is adopted, whereas in rammed earth the ramming process is limited to top surface, thereby creating a varying density profile within the layer. It was also seen that the variation of density within the layer reduces with increase in compaction effort. As the compaction energy changes, the manufacturing water content should also change in order achieve maximum dry density(Beckett & Ciancio, 2014; Smith & Augarde, 2014; B. V. Venkatarama Reddy & Prasanna Kumar, 2011b), hence the influence of manufacturing parameters on the rammed earth is vital in understanding mechanical parameters. Unlike the standardised experimental procedure specified for concrete, there is no conclusive testing procedure to manufacture and test the rammed earth compressive strength (J. E. Aubert et al., 2015; Q.-B. Bui & Morel, 2009; D. Ciancio & Augarde, 2013; Maniatidis & Walker, 2008; J. Morel et al., 2007).
al., 2007). Proctor compaction energies are considered to be more suitable to geotechnical works and has very less relevance for earthen construction (Mesbah, Morel, & Olivier, 1999). To overcome this ambiguity and in the absence of suitable measurable compaction energy to manufacture specimens that can replicate in situ conditions, (Gerard et al., 2015; Hall & Djerbib, 2004; Peter Walker et al., 2005) proposed a technique which resemble in-situ compaction effort. This technique states that the moist soil poured into the formwork has to be compacted until ringing sound is heard upon the impact of hammer on the surface of the compacted soil layer. Similarly to identify the manufacturing water content of the soil, (Maniatidis & Walker, 2003) proposed the drop test to identify the required water content. Considering the above two methods to be very perspective and depended on the mason, many doubts were raised on the reliability and reproducibility (Smith & Augarde, 2014).
Since, it is difficult to replicate the specimens with the exact nature of in-situ walls, and also considering huge variable factors on manufacturing water content and compaction energy. In this study, the cylindrical specimens that are manufactured using Proctor method at three different compaction energies are experimentally investigated for their compressive behaviour. The experiment is focused on studying the reliability of Proctor method for manufacturing specimen. The compressive stress strain characteristic such as, initial tangent modulus and average cyclic modulus are studied by inducing loading and unloading cycles at different stress levels. The influence of dry density and compaction energy on compressive strength and modulus are also presented.
4.2. Experimental studies on rammed earth: a review
Considering that the mechanical testing principle and procedure for both USRE and SRE (cement and lime) to be similar. The literature review of most relevant works on USRE and SRE is discussed below.
of 1.95g/cc to 1.99g/cc. For compression test, cylindrical specimens with dimension of 50mm in diameter and 100mm in height were used, whereas to accommodate necking effect in tensile test at the mid height, specimen length was increased to 140mm high with trimmed diameter at mid height. For cyclic loading, two stress points were predefined one at 40-50% of peak stress and the other at 80% of the peak stress, peak stress was found in monotonic loading. Unconfined compression test was carried out at an axial strain rate of 1%/mm, while unconfined tensile test was carried out at 0.01%/mm for monotonic loading, and 0.05%/mm for cyclic loading. From this experimental investigation initial tangent modulus, secant modulus, peak stress (compressive strength), influence of drying period on compressive strength, relation between tensile strength and compressive strength were studied. The average peak strength of the soil for different series depending on type of curing varied from 2.8MPa to 4.2MPa, with average initial and average secant modulus of 2500MPa and 1000MPa (data extracted from graph - approximate values). The tensile strength was found to be 10% of compressive strength, but the initial tangent modulus in tensile test was similar to compressive test. It was also noticed that the strength and modulus of the material increases with decrease in strength, which is attributed to suction effect. It is interesting to note that the secant modulus is less than initial tangent modulus.
The effect of moisture content on the mechanical strength of the rammed earth was studied by (Q. Bui et al., 2014). In this study, compressive strength, suction effect, elastic modulus of 5 different soils was studied. Cylindrical specimens with aspect ratio of 2 were used to study compressive strength characteristics of the specimens. To study the elastic property of the material, specimens were subjected to cyclic loading pattern. The initial modulus and secant modulus of the specimens were also calculated. From the compressive stress train characteristics, author describes that the material has a linear elastic region up to 15% of the peak stress. From the interpretation of the experimental results, the compressive strength of the specimens increased with the decrease in moisture content, but the rate of increase in strength varied with change in soil. The compressive strength of USRE soil specimen’s was in quasi static state for less than 4% moisture content. Using filter paper technique, suction strength of the USRE specimens were measured and a relation of suction with respect to compression strength was also established.